To What Extent Does the Zintl-Klemm Formalism Work? The Eu(Zn1-xGex)2 Series
Tae-Soo You; Sven Lidin; Olivier Gourdon; Yaqiao Wu; Gordon J. Miller; Inorganic Chemistry 48 (2009) 6380–6390; doi:10.1021/ic900628k

data_4302712
_publ_section_title
;
To What Extent Does the Zintl-Klemm Formalism Work? The
Eu(Zn1-xGex)2 Series
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6380
_journal_page_last               6390
_journal_paper_doi               10.1021/ic900628k
_journal_volume                  48
_journal_year                    2009
_chemical_formula_moiety         'Eu Zn0.6 Ge1.4'
_chemical_formula_sum            'Eu Ge Zn'
_chemical_formula_weight         289.92
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           191
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   4.2514(4)
_cell_length_b                   4.2514(4)
_cell_length_c                   4.5363(6)
_cell_measurement_temperature    273(2)
_cell_measurement_theta_max      36.0
_cell_measurement_theta_min      4.5
_cell_volume                     71.006(13)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      273(2)
_diffrn_measured_fraction_theta_full 0.989
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measurement_device_type  'Bruker SMART APEX CCD'
_diffrn_measurement_method       'w/ scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0355
_diffrn_reflns_av_sigmaI/netI    0.0173
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            1037
_diffrn_reflns_theta_full        35.23
_diffrn_reflns_theta_max         35.23
_diffrn_reflns_theta_min         4.49
_exptl_absorpt_coefficient_mu    40.335
_exptl_absorpt_correction_T_max  0.923
_exptl_absorpt_correction_T_min  0.285
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    6.780
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             125
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.335
_refine_diff_density_min         -0.603
_refine_diff_density_rms         0.144
_refine_ls_extinction_coef       0.024(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.219
_refine_ls_matrix_type           full
_refine_ls_number_parameters     6
_refine_ls_number_reflns         89
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.219
_refine_ls_R_factor_all          0.0109
_refine_ls_R_factor_gt           0.0109
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0000P)^2^+0.0763P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0248
_refine_ls_wR_factor_ref         0.0248
_reflns_number_gt                89
_reflns_number_total             89
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic900628k_si_001_4.cif
_cod_data_source_block           EuZn0.6Ge1.4
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_database_code               4302712